5.66k likes | 10.17k Vues
Testing of materials. Damian Keenan Sept 2010. There are two main categories of materials testing; 1. Destructive Testing 2. Non-destructive Testing. The types of destructive tests used in Engineering are; Tensile Test Hardness Test Toughness Test Creep Test Fatigue Test.
E N D
Testing of materials Damian Keenan Sept 2010
There are two main categories of materials testing; • 1. Destructive Testing • 2. Non-destructive Testing
The types of destructive tests used in Engineering are; • Tensile Test • Hardness Test • Toughness Test • Creep Test • Fatigue Test
The types of non-destructive tests used in engineering are; • Visual Inspection • Dye Penetrant Test • Magnetic Particle Test • Eddy Current Test • Ultrasonic Test • X-Ray Test
Tensile Testing • Tensile testing involves the stretching of a piece of material, or putting it under strain, and examining how it behaves under test. • The ductility of a metal can be found by tensile testing using an extensometer, which is an instrument for measuring the amount that a specimen stretches or extends during a test.
These specimens may be rectangular or circular but must have a specified cross sectional area (CSA). • They also must have punch marks a specified distance apart (Gauge Length).
The Test Procedure • The specimen is set up in the tensile testing machine, the extensometer. • One end is held in a vice and the other in a holding system. • A controlled load, measured in newtons (N), is applied. • The amount of stretch or extension that this force causes is measured.
A material that returns to its original length has elasticity. Repeated test are carried out making the load greater each time. • While the material under test has elasticity the extension or stretch is directly proportional to the load. • This is known as Hookes Law. Metals are elastic in the early stage of tensile testing, plastics are not.
When a material fails to return to its original length it has reached its elastic limit or limit of proportionality. • After the elastic limit the loads produce much larger extensions of the specimen. This is called the plastic region. • At the end of this stage, the extension is even greater and a yield point is reached.
A further increase in the load causes the specimen to thin uniformly and then to neck. After necking the specimen will break or fracture. • When the fracture occurs one side of the specimen has a rough cone shape and the other has a rough cup shape. • This is known as a cup and cone fracture
Stress • Stress can be defined as the amount of load or force carried by a unit area. It is normally written as Newtons per millimetre squared, (N/mm2). • Stress = Load Cross Sectional Area (CSA)
If a bar, 15mm wide X 8mm deep, is pulled with a force of 360 kN, the stress is found as follows. Force = 360 kN Cross Sectional Area (CSA) = 120 mm2 (15mm X 8mm) Stress = 360kN 120mm2 = 3 kN/mm2
Young’s Modulus of Elasticity In the elastic range of a material, stress is directly proportional to strain, which is another way of stating Hookes Law. This is called Young’s Modulus, is represented by ‘E’ and measured in kN/mm2.
Tensile StrengthTensile strength is the maximum force of load, in Newtons, applied to the specimenbefore it fractures divided by the original cross sectional area.
Proof Stress • Some materials do not have a well defined yield point or an indication at what stress yield occurs. • To overcome this, a value of stress, known as proof stress is used.
Reading 0.1% Proof Stress from a force-extension graph • A distance equal to 0.1% of the gauge length, from the origin, is located. • If the gauge length is 56mm, then the distance from the origin for 0.1% proof stress is 0.056mm • A line, parallel to the straight part of the graph, is drawn from the 0.056mm mark until it cuts the graph line. • The stress at that point is the 0.1% proof stress.
Reading 0.1% Proof Stress from a stress-strain graph • Proof stress is much easier to find from a stress-strain graph. Proof stress is read almost directly from this type of graph • If the 0.1% proof stress is required, then a line is drawn from 0.001 strain, parallel to the straight part of the graph.
Youngs Modulus of Elasticity = Stress / Strain Stress = Load / CSA = 50 / 78.5 = 0.64 Strain = Extension / Original Length = 0.2 / 50 = 0.004 Youngs Modulus of Elasticity = Stress / Strain = 0.64 / 0.004 = 160 kN / mm2
Hardness of Materials • Hardness is tested by measuring the material’s resistance to indentation or scratching of its surface. • Hardness in metals may vary or can be changed by heat treatment.
1. The Brinell Test, which uses a ball indenter • 2. The Vickers Test, which uses a diamond, square based pyramid indenter • 3. The Rockwell Test, which uses a steel ball for soft materials and a diamond cone for hard materials
The Brinell Test • Indenter:Hardened steel or Tungsten Carbide ball, • Procedure:Ball indenter forced into the surface of the test piece by a suitable load. • Diameter of indentation is measured and converted into a Brinell hardness number. • The test piece must be 8 times thicker than the depth of the impression to prevent the table of the test machine absorbing the indenting force.
Uses: Used on iron castings and drop forgings. • Disadvantages: Cannot be used on thin material specimens. • Ball deforms with very hard material specimens. • Ball indents too much with soft material specimens
The Vickers Test • Indenter: Diamond, square based pyramid – point angle of 136° • Procedure: Diamond indenter forced into the surface of the material being tested making a square shaped impression. • The diamond pyramid is less likely to distort under high forces than the steel ball.
The diagonal length of the impression is measured and this measurement is converted into a Vickers hardness number. • The test piece must be 5 times thicker than the depth of penetration required. • Uses – Used for very hard materials, gives a more accurate reading than Brinell. • Easier to use. A smoother surface is required on test pieces, which makes this method ideal for finished components
The Rockwell Test • Indenter: The two most common indenters are the Ball and Cone. • Procedure:Similar to the Vickers process. • Rockwell system has a large range of hardness scales. • Each scale has its own type and size of indenter, as well as a specified indenting force. • ‘C’ scale indicates that a Cone was used and ‘B’ scale indicates that a Ball was used. The ball is used for soft materials and the cone is used for hard materials.
Note: Both the Brinell and Vickers hardness tests measure the surface areas that the indenters make, to determine the hardness numbers. but the Rockwell test measures how far the indenter moves into the material being tested.
Toughness Testing • Toughness testing can also be called Impact Testing or Notched Bar Testing. • The two common methods of Impact testing are • The Izod Test • The Charpy Test